JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
available at www.sciencedirect.com
journal homepage: www.elsevier.com/locate/jmbbm
Marc A. Meyers∗, Po-Yu Chen, Maria I. Lopez, Yasuaki Seki, Albert Y.M. Lin
University of California, San Diego, La Jolla, CA, United States
Article history: The approach used by Materials Science and Engineering is revealing new aspects Received 25 May 2010 in the structure and properties of biological materials. The integration of advanced Received in revised form characterization, mechanical testing, and modeling methods can rationalize heretofore 20 August 2010 unexplained aspects of these structures. As an illustration of the power of this Accepted 22 August 2010 methodology, we apply it to biomineralized shells, avian beaks and feathers, and fish scales.
We also present a few selected bioinspired applications: Velcro, an Al2O3-PMMA composite inspired by the abalone shell, and synthetic attachment devices inspired by gecko. ⃝c 2010 Elsevier Ltd. All rights reserved.
1. Introduction and basic components ...... 1 2. Hierarchical nature of biological materials ...... 3 3. Structural biological materials...... 5 3.1. Abalone shell ...... 5 3.2. Toucan and hornbill beaks...... 14 4. Functional biological materials...... 17 4.1. The gecko foot ...... 18 4.2. Tree frog...... 20 4.3. Abalone foot attachment ...... 21 5. Bioinspired materials and structures...... 23 6. Conclusions ...... 29 Acknowledgements ...... 29 References ...... 29
1. Introduction and basic components distinct but interrelated components: • Biological Materials: natural materials • Biomaterials: synthetic materials in biomedical applica- Biological Materials Science is a new and rapidly growing tions branch of Materials Science and Engineering. It has three • Biomimetics: bioinspired materials and design
✩ Dedicated to the memory of Mia Tegner, who kept the abalone used in our research and died in a tragic diving accident, after spending her career as marine biologist studying abalone, who lives through them. ∗ Corresponding author. Tel.: +1 858 534 4719; fax: +1 858 534 5698. E-mail address: firstname.lastname@example.org (M.A. Meyers). 1751-6161/$ - see front matter ⃝c 2010 Elsevier Ltd. All rights reserved. doi:10.1016/j.jmbbm.2010.08.005 2 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Table 1 – Principal components of biological materials.
Hard component: minerals Soft component: organic macromolecules
Calcium carbonate (CaCO3) Collagen (Types I, II,. . . , XXVIII) Calcium phosphate (hydroxyapatite, Ca10(PO4)6(OH)2) Keratin Silica (SiO2) Chitin Magnetite (Fe3O4) Elastin Copper oxide Cellulose Resilin and Abductin
There is overlap between these three components. For • Many components serve more than one purpose; for instance, biological materials have been successfully used in instance, the skin protects the organism and regulates the a number of biomedical applications. Examples are biological temperature; bone is a structural component as well as a scaffolds, coral used in bone regeneration, collagen used in factory for red blood cells. Thus, the structures are called implants, etc. (e.g. Stella et al., 2010). ‘multifunctional’. The prominence of this field can be assessed by the three • The properties are highly dependent on the level of water international conferences on Mechanics and Biomaterials in the structure. There are some remarkable exceptions, & Tissues (2005, 2007, 2009), organized by the Journal of such as enamel, but this rule applies to most biological Mechanical Behavior of Biomedical Materials, by the yearly materials and is of primary importance. • Biological Materials Science Symposia held at the Annual Evolution, environmental constraints, and the limited availability of materials dictate the morphology and TMS-AIME meetings (2006–2010), and by the number of properties. The principal elements available are oxygen, sessions and symposia dedicated to this theme at the nitrogen, hydrogen, calcium, phosphorous, silicon, and Materials Research Society meetings. carbon. In addition, trace elements (e.g. Fe) have been There have also been a number of overview articles found to be crucial for phase determination in some presenting the field in a broad manner. Noteworthy among systems, for example, iron oxide in radular teeth of them are overviews in Progress in Materials Science (Meyers chiton (Saunders et al., 2009; Weaver et al., 2010). The et al., 2008a) and in JMBBM (Chen et al., 2008a), and most useful synthetic metals (iron, aluminum, copper) are articles dealing with broader aspects of biomineralization virtually absent and are only present in minute quantities (Lowenstam and Weiner, 1989; Mann et al., 1993; Weiner and highly specialized applications. The processing of and Addadi, 1997; Mann, 2001; Ehrlich, 2010) and structural these elements requires high temperature processes not biological materials (Vincent and Currey, 1980; Vincent, 1991; available in natural organisms. Mayer, 2005; Meyers et al., 2006; Fratzl and Weinkamer, 2007; • Except for a few remarkable exceptions, the synthesis Chen et al., 2008b; Buehler et al., 2008; Espinosa et al., 2009; of biological materials is conducted in an aqueous McKittrick et al., 2010). The book Collagen edited by Fratzl environment at ambient temperature and pressure of 1 (2008) presents a comprehensive treatment on the subject. atm. This article will focus primarily on recent research carried • The structures are hierarchical, i.e., they have different out by our group as well as on a few selected biomimetic scale levels conferring distinct properties. applications. Table 1 shows the principal components of biological It is important to emphasize that some knowledge of materials. They can be divided into two groups: organic biology is also important. Significant misunderstandings can materials and biominerals. Organic materials that can be arise if researchers are ignorant of, for example, animal likened to polymers in MSE, provide, for the most part, a anatomy and physiology, the lifestyle of animals (since greater ability to undergo deformation, whereas the minerals their activities determine the applied loadings) and cell sustain loading. The organic components can be extended in biology/biochemistry which determines how structural parts tension, whereas the ceramic resists primarily compression are created and maintained. In an analogy, the same potential (e.g., tooth enamel). Few biological systems are subjected to errors can arise when materials scientists working on uniaxial tension (exceptions being ligaments and tendons), engineering projects proceed without an understanding of but flexure is a common mode of loading. In flexure, one the engineering structures in which their materials will be half of the cross-section is subjected to compression and the used in. other half to tension. It is only in rare occasions that minerals Biological materials and structures have unique charac- are not present in combination with organic materials. The teristics that distinguish them from synthetic counterparts. organic components, in turn, have a wide variety of structures These are shown in the schematic (Arzt, 2006) figure, ex- that confer uniaxial, biaxial, or triaxial properties. panded to a hexahedron. The six components are presented The basic molecular units of the organic components below: are amino acids organized primarily into polypeptides and polysaccharides. Polysaccharides are the building blocks of • The structures are assembled from the bottom-up, rather cellulose and chitin. Polypeptides form proteins. Proteins than from the top-down. This is a necessity of the growth are prominent in mammals and comprise most of the process, since there is no availability of an overriding extracellular material. The principal protein in mammals scaffold. This characteristic is called ‘self-assembly’. is collagen, a fibrilar organic molecule. The basic structure JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 3
have 4–8. In synthetic materials the mechanical strength is designed into the structure primarily at the micrometer and millimeter levels. On the other hand, the elastic modulus is the direct result of inter-atomic bonding, which operates at the nanometer level. Hence, the grains in metals and the fiber bundles in composites are the principal hierarchical levels. Biological materials also have an important difference: self-healing capability, enabled by the cells extant in the extracellular material. Thus, the material can recover its original properties. There is a complex interplay that takes place between the different levels of hierarchy that will be analyzed later in this section. In previous reviews, we have presented the hierarchical structure of abalone (Lin and Meyers, 2005), crab exoskele- ton (Chen et al., 2008c), antler (Chen et al., 2009; Launey et al., 2010a), horn (Tombolato et al., 2010), all studied by members of our group. We illustrate this concept here for two addi- tional materials, avian feather and fish scales. Fig. 3(a) shows a schematic of a feather and several SEM micrographs at in- creasing magnifications. The feather rachis (central shaft) has a cellular core contained in a solid envelope. Both are keratin. The internal foam has a fascinating structure. It consists of cells with approximate diameter of 10 µm, in the case of the Fig. 1 – Schematic representation of characteristic Falco sparverius primary remiges (flight feathers located on the constraints/components in the study of biological systems. posterior side of the wing) shown in Fig. 3(a). If one images the Source: Modified from Arzt (2006). cell walls at a higher magnification, one recognizes that they are not solid but are, in turn, composed of fibers with a diame- starts with three polypeptide chains forming a triple helix. ter of ∼200 nm, as shown in Fig. 3(b). Thus, one has a two-level These polypeptides contain repeating amino acid motifs (Gly- cellular structure that minimizes, as required, weight. The ad- X-Y) where X and Y can be any amino acid. The chains vantage, in terms of density, of having a two-level hierarchy form right-handed helices and the glycine residues are on in the cells, is readily obtained from: the inside of the helix, whereas the X and Y amino acids ρ t 2 are exposed, on the outside. The macromolecular units For level I, I = C 1 (1) ρ 1 l have approximately 300 nm length. Fig. 2(a) shows the II 1 2 polypeptide chains forming tropocollagen and the collagen ρII t2 For level II, = C2 (2) units bonding in a head-to-tail arrangement, with gaps and ρs l2 overlap regions. The macromolecules are attached to each where ρI is the density of the cellular structure at level I, ρII other and the terminations form gaps that reveal themselves, is the density of the porous strut, and ρs is the density of in transmission electron microscopy, by the characteristic the solid material, respectively. There are two characteristic banded pattern with a repeat distance of 64–67 nm. This is dimensions: the cell size, l, and the strut thickness, t. C1 and the stagger distance between adjacent molecules. Fig. 2(b), (c) C2 are proportionality constants. show the characteristic pattern revealed in antler collagen. The fibrils have a diameter of 100 nm. They assemble ρ t t 2 Thus, I = C 1 2 . (3) themselves into fibers and other arrays that can be one, ρs l1l2 two, or tridimensional. Fibrilar collagen (Types I, II, II, V, XI, XXIV, and XXVII) is the most important of the over 20 types If the two levels are geometrically similar, t1/l1 ≈ t2/l2 ≈ of collagen in humans: Type I is the most common, found t/l, and: primarily in skin, tendon, bone, lung, and arteries/veins; Type ρ t 4 II, in cartilage; Type III, found in very elastic tissues. Collagen I = C . (4) ρ has been called, very appropriately, the ‘steel’ of biological s l materials by Fung (1993), not because of its properties but Thus, the relative density ρI/ρs varies as the fourth order because of its multiple and diverse applications. of the geometric ratio t/l. This is indeed a very strong dependence. Fig. 4 shows the hierarchy of the scales in a large river 2. Hierarchical nature of biological materials fish, the Arapaimas gigas. This fish can weigh as much as 200 kg. It lives primarily in Amazon basin lakes. It This is a unique aspect that defines biological materials, is covered with scales having up to 10 cm length. These as seen in the hexagon of Fig. 1. One can also think scales have a collagen interior with a highly mineralized of synthetic materials as hierarchical, but in many cases external layer. The mineral phase is non-stoichiometric they only have 2 or 3 levels, whereas biological materials hydroxyapatite, the same as that in bones. The collagen 4 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 2 – (a) Collagen structure, starting with three polypeptide chains forming units ∼300 nm long. Overlaps and gaps generate characteristic pattern with 64–67 nm periodicity (b) TEM micrograph of a Type I collagen fibril obtained from demineralized elk antler showing characteristic 67 nm periodicity; (c) Maximum intensity projection (MIP) assembled from series of TEM images showing the structural organization of collagen fibrils. Source: Courtesy of P.-Y. Chen, unpublished results.
fibers form a cross-lamellar arrangement which produces a and the only difference is the scale. There are two compo- laminate composite structure. This structure can undergo nents: the discontinuous ceramic and the continuous colla- significant non-elastic deformation prior to failure, providing gen phase, in a structure initially proposed by Jäger and Fratzl considerable toughness. The piranha (Serrasalminae) is one of (2000). However, this “Russian doll” hierarchy is also an ap- the principal predators in seasonal lakes, in which fish get proximation, since it assumes that all levels are geometri- trapped. Its teeth form triangular arrays creating a guillotine cally similar. In actual structure, each hierarchical level has action that is highly effective in slicing through muscle. We its own structure, as will become obvious from the discussion performed mechanical tests on the scales and teeth and below. There is significant evidence in the literature that the characterized both (Meyers et al., in preparation). The cutting strength, as measured by hardness, decreases as one marches and puncturing ability of the piranha teeth were evaluated up the spatial scale. The converse is true for toughness, as and it was demonstrated that they cannot penetrate the measured by the ability to resist crack propagation. Fig. 5(b) Arapaimas scales, which provide protection against them shows these combined effects in a schematic manner. The because of the hierarchy of their construction. The ability decrease in strength can be rationalized in a simple manner of the Arapaimas to resist the attack of piranha is clearly by the existence of flaws of greater and greater dimensions the result of the hierarchical structure displayed in Fig. 4, as the sample size is increased. This is a direct consequence consisting of a cross-lamellar arrangement of collagen fibers covered by a highly mineralized external shell. of Weibull statistics. The decrease in hardness is connected The recognition that the hierarchy of the structure is an to the greater availability (or ease of generation) of defects essential feature of biological materials is leading to analyses as the indentation size is increased. In the case of minerals, of a more rigorous nature, beyond the descriptive schemat- the strength reaches the theoretical value (equal to approxi- ics abundant in the literature. The analytical approach de- mately 10% of Young’s modulus) when the scale is reduced to veloped by Gao et al. (Gao et al., 2003; Ji and Gao, 2004; Gao, the nanometer scale. The increase in toughness with increas- 2006; Yao and Gao, 2008) is noteworthy. Fig. 5(a) shows a self- ing scale is a fascinating effect that counteracts the decrease similar hierarchical structure constructed in a simple and in strength. A growing crack will encounter both intrinsic and logical manner: the different levels are geometrically similar extrinsic (in the terminology of Ritchie’s group (Nalla et al., JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 5
t b 1
l1 Level I Level II
Fig. 3 – (a) Schematic of falcon feather along with scanning electron micrographs; (b) Schematic drawing showing two-level hierarchy of open cell structure in feather. Source: (a) Courtesy of S.G. Bodde, unpublished research.
2003, 2005; Yang et al., 2006)) barriers as it propagates. The na- • Level II is composed of the mineral bridges between ture and effectiveness of these mechanisms changes with the tiles, with a diameter of 20–60 nm; it also comprises the hierarchical scale and this explains the toughness increase. sandwich structure of the organic intertile layer, with a The hierarchical levels establish a balance between these two core consisting of a random dispersion of chitin fibrils mechanical properties. and a thickness equal to the length of the mineral bridges ∼ The hierarchical structure of biological materials needs ( 20 nm). • Level III are the well recognized hexagonal tiles, with to be analyzed with a greater emphasis on the mechanisms lateral dimensions of 10 µm and thickness of 0.5 µm. These at the various levels. This is currently only happening tiles are, in general hexagonal, but not always. They also in a few materials. The hierarchy of bone was presented have a distribution of lateral dimensions. by Weiner and Wagner (1998); Rho et al. (1998); Buehler • Level IV are the mesolayers, which are formed by seasonal (2007) as composed of seven levels. For the abalone shell, fluctuations and are characterized by a thick organic layer extensively investigated by our group, one can establish (thickness ∼200 µm) separating tile assemblages with five different levels. The self-similar picture of Fig. 5(a) approximately 0.1–0.3 mm. is an oversimplification, and one cannot invoke the same • Level V is the entire structure that, because of its deformation and failure mechanisms at the different levels. architecture (dome shape, thickness distribution, etc.) is Fig. 6 shows the five levels identified for abalone nacre: optimized for strength and toughness. These two examples (in Figs. 5 and 6) illustrate what needs • Level I is the molecular structure of the chitin fibers that to be done for other hierarchical materials: a quantitative are the structural components of the intertile organic hierarchical structure division into levels, followed by the layers and of the atomic crystalline structure of the analysis of the deformation and failure mechanisms at the aragonite (which might incorporate nanosized islands). different levels. 6 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 4 – 4 Hierarchical structure of the Arapaimas gigas scales. Source: Y.S. Lin et al., unpublished results, 2010.
toucan and hornbill beaks. Our previous overviews in this journal have covered bone, teeth, horn, crab exoskeleton, and antler (Chen et al., 2008a; McKittrick et al., 2010). Table 2 provides an overview of the biological materials under past or current investigation by members of our group.
3.1. Abalone shell
Two aspects of the abalone shell have been investigated: growth and structure/property relations. They are related, i.e., growth determines the structure, which, in its turn, is responsible for its outstanding toughness. Three techniques were used for extracting specimens for growth observations: the flat pearl, the trepanning techniques described by several groups (Fritz et al., 1994; Belcher et al., 1996; Shen et al., 1997; Meyers et al., 2008b; Lin et al., 2008), and a simpler method, which consists simply of removing a wedge of the shell and observing it (Meyers et al., 2009). The trepanning and flat pearl (glass slide) techniques gave equivalent results, which are shown in the sequence of Fig. 7. The central picture is a cross-section (fracture) of the shell. The growth proceeds from bottom to top. The bottom part is a thick organic mesolayer; it is characteristically smooth. Fig. 5 – Schematic drawings (a) showing self-similar The reinitiation of growth after a prolonged period of rest hierarchy (analogous to a Russian doll) with levels I, II,. . . , takes place in stages. First, columnar aragonite crystals are N ; (b) strength and toughness as a function of number of formed with the fast growth direction (c-axis), pointing up. hierarchical levels. These crystals radiate from the nucleation sites and form a Source: (a) Adapted from Gao (2006). characteristic spherulitic pattern. Eventually, the tile growth pattern replaces it, shown on the top of the central picture. The same sequence occurs when a glass slide is applied 3. Structural biological materials to the growing surface of the abalone and removed after predetermined periods of time. Fig. 7(b) shows an array of We will focus in this section on two biological systems that such slides glued to the growth surface of the shell. They are we have investigated in detail, the abalone shell and the readily covered by the mantle after the animal is returned to JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 7
Fig. 6 – Hierarchical structure (5 levels) of the abalone nacre from nano, micro, to meso to structural length scales.
Table 2 – Principal biological materials investigated at UC San Diego in the period 2000–2010.
Mammal Fish Bird Invertebrates
Teeth and Tusks Scales-Arapaimas Beaks Mollusk shells — hippo Teeth — piranha — toucan — abalone — warthog — shark — hornbill — conch Armadillo carapace Feather — clam Antlers and Horns Claw Arthropod Skin Exoskeletons — crab — horseshoe crab Sponge spicules 8 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 7 – (a) Sequential growth of abalone nacre from flat pearl experiment; (b) Glass slides (depicted by arrows) embedded in abalone shell; flat pearl technique. Source: (a) Adapted from Lin et al., Acta Biomater. (2008); (b) Adapted from Lopez et al., MSEC (in press). water and mineralization takes place on them. This is shown the abalone. Fig. 8 shows sequential growth results 1 week for intervals varying from 1 to 6 weeks in the peripheral after implantation (Lopez et al., in press). Tile growth takes pictures of Fig. 7(a). These pictures represent top views place at 21 ◦C when abalone was regularly fed (Fig. 8(a)). The taken from flat pearls. After 3 weeks, the columnar growth formation of tiles is reestablished after 1 week. The growth is still predominant. However, at six weeks a remarkable cones can be seen under the organic layer that completely change has taken place: growth cones are observed, under sagged upon removal of sample from water. In contrast, an organic layer. More recent experiments indicate that the ◦ transition time to tile growth is dependent on the outside growth at 15 C with abalone regularly fed still shows the ◦ conditions. The growth in colder water is sluggish and the columnar pattern (Fig. 8(b)); similarly, growth at 20 C without transition is slow. Another noticeable effect is the feeding of food available is also columnar (Fig. 8(c)). JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 9
Fig. 8 – Sequential growth result 1 week after implantation. (a) Growth at 21 ◦C and abalone was regularly fed; (b) Growth at 15 ◦C with abalone regularly fed; (c) Growth at 20 ◦C without food available. Source: Adapted from Lopez et al., MSEC (in press).
Fig. 9 – Growth surface in red abalone (coated specimen, high vacuum SEM): (a) overall view showing mineral apexes and flat organic layer; (b) cracked organic layer; (c) detailed view of three terraced growth sequences; (d) top viewoffractured terraced growth sequences exposing incompletely grown tiles with central holes. Arrow in (c) denotes central core orifice revealed by fracture of terraced cone. Source: Adapted from Meyers et al., MSEC (2009).
The details of this growth pattern are much more clearly organic layer breaks the cones which are seen in Fig. 9(c) seen in Fig. 9. Fig. 9(a) was taken with the environmental (sideways). In Fig. 9(d) the tops of the growth cones were mode of the SEM; the top organic layer (‘canopy’) is cracked, removed and the base tiles are shown. Each one has a hollow revealing the growth of the cones (“Christmas tree” pattern) core; there is still some disagreement as to the origin and underneath. Using the high vacuum mode leads to drying function of the hollow core. Whereas Meyers et al. (2009) of the organic layer and shrinkage, resulting in extensive hypothesized that this was due to simultaneous growth of cracking. The mechanical response of this layer is radically altered by the removal of water; it becomes hard and brittle. three or more new tiles at each layer, leaving a depleted This was indeed fortuitous and enabled the clear observation region in the center, Checa et al. (2009) suggest that there of the growth cones, Fig. 9(b). In places, the shrinking of the is a growing central organic-rich core. In a counterargument, 10 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 10 – Atomic force microscopy of green abalone in tridimensional representation: arrows denote boundary between successive layers in stacks (terraced cones). Section analysis of abalone mineral tiles protruding from surface along line indicated in the micrograph (vertical distances between lines ∼500 nm). Source: Adapted from Meyers et al., MSEC (2009).
Meyers et al. (2009) show specimens where this central core By demineralizing the shell using 0.6N HCl, it was possible is absent. to image the central core of the organic layer (Fig. 12(a)). It The same growth surfaces were imaged by AFM and the consists of chitin fibrils having a diameter of ∼20 nm. They growth cones are shown as light regions in Fig. 10. A depth had been previously imaged by AFM and the SEM picture trace was made along the line marked on the right-hand confirms their structure. The chitin network provides the side. It shows the characteristic 500 nm steps that correspond mechanical strength to the organic layer. The chitin core is to the thickness of the tiles. Arrows show the steps in the surrounded by acidic macromolecules that attach themselves perspective view. to the top and bottom surfaces of the tiles (Fig. 12(b)) (Sarikaya The organic layer is imaged by SEM in Fig. 11(a). It has holes et al., 1990; Checa et al., 2009). that have approximately 20–60 nm in diameter. These holes It was possible to establish, in a preliminary and semi- enable the continuation of growth from one layer to the next quantitative manner, the mechanical strength of the organic interlayer. When the samples are imaged without any and the formation of bridges, which will be discussed below. preparation, the organic layer can be seen sagging deeply They also ensure that the same crystallographic orientation between the cones. The sag was used to estimate the strength is maintained from layer to layer in the same stack. Fig. 11(b) of the wet layer, considering that only its weight is acting on shows the growth mechanism as is thought to occur. The it. This resulted in extremely low values of the flow stress, animal periodically creates and deposits the organic layer, suggesting that the organic is viscoelastic and flows under its whose core is composed of chitin fibers. Growth in the weight when removed from water, which supports it under c-direction is arrested but eventually restarted once the normal growth conditions. In stark contrast with these initial crystal can penetrate and traverse the holes. The membrane − measurements (Meyers et al., 2008b), the nanoindentation is permeable to Ca2+ and CO2 ions and lateral growth 3 method was used to penetrate the dry organic layer (Meyers can therefore take place after a membrane is deposited. et al., 2009) and encountered considerable resistance. This Eventually the lateral growth of the tiles is arrested when they was a trial-and-error procedure in which the Berkovich impinge upon each other. It is interesting to note that the indenter was lowered and touched, in a large fraction of the lateral organic layer between tiles at the same height (arrow attempts, the organic layer. The configuration used in testing B) is less visible than the top ones (arrows A). The SEM inset in is shown in Fig. 13. One considers that the membrane is held Fig. 11(b) shows this through backscattering. This is in perfect up by three growth cones. When the Berkovich tip with a agreement with recent results by Checa et al. (2009) and triangular base and angle of 136◦ is lowered, it may touch the dismisses the idea of a preexisting three-dimensional scaffold organic before it encounters the mineral, situations depicted as a figment of the imagination. In region B we probably have in Fig. 13(b) and (c). In this case, the load–penetration curve remains of organics pushed out by the lateral growth fronts. shows drastic changes from the ones in which the tips of This is analogous to the zone refining process in metallurgy, the cones are encountered first. Actual curves are shown in where the concentration of impurities in the liquid gradually Fig. 14. Fig. 14(a) shows that the force rises rapidly as the increases as the solidification process advances, expelling the tip of the two cones are deformed. In one of the cases, the impurities. tip breaks, creating a characteristic displacement. For the JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 11
Fig. 11 – (a) SEM image showing thin intertile organic layer with holes ; (b) Proposed mechanism (Lin and Meyers, 2005, MSEA; Meyers et al., 2009, MSEC) of growth of nacreous tiles by formation of mineral bridges; organic layer is permeable to calcium and carbonate ions which nourish lateral growth as periodic secretion and deposition of the organic intertile membranes restricts their flux to the lateral growth surfaces. In inset (SEM Backscattering mode) Fig. 12 – (a) Demineralized shell revealing randomly the intertile organic layer is visible as dark horizontal lines oriented chitin fibrils from intertile layers; (b) schematic (A), while regions where tiles abutt (vertical lines) are representation of organic intertile layer composed of chitin barely seen (B), supporting formation of interlayer organic fibrils; (c) chemical structure of chitin. layers to regulate growth. Source: Adapted from Lopez et al., MSEC (in press). Source: (a) From Lopez et al., MSEC (in press) (b) Adapted from Meyers et al., MSEC (2009).
where more detailed analysis is needed to establish the effect other situation (Fig. 14(b)), there is a plateau at P ∼ 100 µN, of the organic layer hydration on its mechanical response. corresponding to the resistance of the organic layer. This How does the abalone produce the organic interlayer penetration proceeds, for three curves, for approximately at periodic intervals? We excised a portion of the mantle, 300 nm. Considering some sag in the organic layer, this and examined its section, and particularly the region in number represents one tile layer. One of the curves has a close contact with the growth surface. Observation of the more extensive plateau, around 600 nm. In this case, it is inner layer of the epithelium, which is only separated thought that the indenter travels the distance of two layers, from the growth front by the extrapallial layer, revealed as shown in Fig. 13(c). These measurements were used to interesting features. This epithelium contains arrays of estimate the resistance of the organic layer to deformation channels, Fig. 15(a). In some of these channels a few fibrils and/or failure. There was a drastic increase in strength from are seen and marked with arrows. Thus, one can envisage the original values obtained by measuring the sag in the the synthesis of chitin in the channels and its periodic membrane, attributed to the high sensitivity of the structure extraction/extrusion from there onto the growth front. Such on the degree of hydration. This is still an area of research a situation is depicted in Fig. 15(b). 12 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 13 – Representation of nanoindenter deforming b organic layer; (a) tridimensional representation of indenter deforming organic layer; (b) configuration of a single organic layer with a mineral underneath; (c) configuration of an organic layer that is joined with lower level by deflection. Source: Adapted from Meyers et al., MSEC (2009).
Fig. 15 – (a) Cross-section of epithelium with array of channels and occasional chitin fibrils (marked by arrow); (b) schematic depicting hypothetical mechanism by which epithelium generates chitin fibrils and ‘squeezes’ them onto growth surface. Source: Adapted from Lopez et al., MSEC (in press).
The detailed knowledge of the structure at the different hierarchical levels is essential for the understanding of the mechanical properties of nacre. Gao et al. (2003) proposed that, at the nanoscale, the material can reach its theoretical strength because the crack is reduced to the size which is dictated by the scale. This is easily seen by the simplified plot in Fig. 16(a), which shows the stress required to propagate a crack in calcium carbonate, with a fracture toughness 1/2 KIC = 1 MPa m . This curve intersects the line marking the theoretical cleavage stress, approximated as E/30, for a characteristic size of 56 nm. If one looks at the sizes of the mineral bridges joining adjacent mineral layers (Fig. 16(b)), one sees that these are their approximate diameters. Four such bridges are marked by arrows. Fig. 16(c) shows the distribution of tensile strengths obtained by applying tensile Fig. 14 – Nanoindentation load–displacement curves for (a) loads as indicated in Fig. 16(c). They are astoundingly low, completely mineralized region and (b) organic layer in around 3 MPa (Fig. 16(d)). It will be shown below that this green abalone; notice the penetration for ∼400 nm in three is consistent with the calculations based on the observed curves at a low load, before the indenter touches the density of mineral bridges. mineral. Only a small fraction of all asperities form bridges. Indeed, Source: Adapted from Meyers et al., MSEC (2009). Song et al. (2002, 2003) measured the number of these bridges JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 13
Fig. 16 – (a) Maximum fracture stress as a function of the diameter of the mineral bridge (critical flaw size); (b) SEM micrograph showing mineral bridges ∼60 nm between aragonite tiles (marked by arrows) after deproteinization; (c) tensile testing direction perpendicular to tile layers; (d) tensile strength of shells perpendicular to layers. Source: Adapted from Lin and Meyers, JMBBM (2009). per tile and found approximately n = 40. These numbers are large tensile strength when pulled along the direction of the in agreement with the simple calculation shown here. tiles. We recognize that the shell is not subjected to tension The tensile stress, σt, is equal to the sum of the forces in this direction in its natural habitat. Nevertheless, tension is exerted by n mineral bridges divided by the area of a tile, involved in bending, a stress that is definitely involved when At. The force per bridge is equal to the theoretical stress, σth, a predator pries it from a rock. Flexure tests show values multiplied by the bridge area, Ab. Thus: of 170 MPa, compared with a compressive strength of 235 nA σ MPa, in the same orientation. Dog-bone shaped samples were = b th σt . (5) also used to determine the tensile strength of nacre when At loaded parallel to the plane of growth; the mean strength was Taking the tile radius as 5 µm, the number n = 40, the considerably lower, 65 MPa. Nevertheless, the tensile strength theoretical strength (Fig. 16(a)) σ = 3.2 GPa, and the diameter th is a much higher fraction of the compressive strength (1/4– of the bridges equal to 60 nm, one obtains: 1/2) than in monolithic ceramics, where it fluctuates between σt = 1.2 MPa. 1/10 and 1/15. The failure occurs by the process shown in This is on the same order of magnitude as the mean from the the SEM micrograph of Fig. 17(a): the tiles pull out and are only occasionally broken. On the other hand, if the bonding Weibull distribution in Fig. 16(d) (σt = 3 MPa). One can also expect the organic layer to contribute with bonding between between tiles were stronger, they would crack and allow adjacent layers. It should be mentioned that Kamat et al. the propagation of a crack that could cross the specimen (2000, 2004) took exception to the Gao et al. (2003) analysis. unimpeded. Shear tests were conducted on a special fixture They attributed the strength to micrometer-scale features. with a shear gap of 200 µm, approximately 100 µm narrower These results are indeed significant and indicate that than the spacing between mesolayers. Fig. 17(b) shows how the mineral bridges play a seminal role in the mechanical the tiles slide past each other. Assuming that the majority properties of the abalone shell. Lin and Meyers (2009) of failure occurs through tile pull-out and not through tile extended this treatment to the tensile and shear strength and fracture, the tensile strength can be converted into shear obtained consistent values. The most important attribute of strength. Indeed, we measured the average pull-out strength nacre, its high toughness, is a direct result of the relatively of tile segments in tension (Lin and Meyers, 2009). 14 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 17 – Origin of toughening in nacre: (a) SEM micrograph showing sliding of tiles in tensile loading; (b) balance between tile fracture and intertile shear; (c) details of three mechanisms of intertile shear: asperities, organic layer acting as viscoelastic glue, and fracture of mineral bridges. Source: Adapted from Lin and Meyers, JMBBM (2009).
There are three principal mechanisms contributing to the The shear strength is found to be 36.9 ± 15.8 MPa with an strength of the abalone shell, shown in the insets of Fig. 17(b): average maximum shear strain of 0.3. Assuming a fracture mineral bridge breaking, asperities, and the bonding provided toughness of 1 MPa m1/2, one can obtain a critical crack size by the organic interlayer. These three mechanisms are shown that will be arrested by the sliding of tiles. in more detail in Fig. 17(c). In conclusion, the layered structure of the abalone shell Taking the equilibrium of forces in Fig. 17(b) the provides anisotropy of mechanical strength that increases relationship between the tensile stress on tile, σt, and shear the toughness in a very significant manner by increasing the stress on organic interfaces, τs, can be calculated for a simple resistance to crack propagation perpendicular to the surface two-dimensional case: and decreasing it correspondingly parallel to it.
F1 = F2 + F3 (6) 3.2. Toucan and hornbill beaks σtt = 2τsS (7) where σt is the tensile strength of the tile and τs is the shear Whereas birds usually have either short and thick beaks or strength of the intertile layer. S is the mean overlap between long and thin beaks, toucans have long and thick beaks. The tiles and t the tile thickness. From Fig. 17(a) one can estimate Toco Toucan (Ramphastos toco) has the largest beak among the mean overlap between tiles: S = 0.63 µm. Their thickness the species. The large beaks help in picking up fruits at the is t = 0.5 µm. Thus, one obtains: tips of branches in the canopy and extracting prey (little baby birds!) from holes in trees. They also assist in combat and σ /τ = 2S/t = 2.5. (8) t s bill fencing. The Toucan beak is one-third of total length of For the abalone tile configuration, the tensile strength of the bird; nevertheless the weight is 1/30th–1/40th of its mass. the mineral should be at least equal to 2.5 times the shear The African Hornbill also has an extraordinarily large beak; strength of the interface to ensure shear failure by sliding. it is, however, heavier. This is accomplished by an ingenious JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 15
Fig. 18 – Photographs and schematic drawings of (a) toucan and (b) hornbill beaks. Source: (a) Adapted from Seki et al., Acta Mater. (2005), (b) Adapted from Seki et al., Acta Biomater. (2010). solution, enabling a low density and sufficient rigidity. The and trabecular rods are made from the same materials, we outside shell (integument) of the beak consists of β-keratin, measured the mechanical properties separately to take into that is typically found in avian and reptilian species. The account the anisotropy of the trabeculae and cortical shell. inside is filled with a cellular bone. This internal foam has For obtaining the response to stresses of the foam at the a closed-cell structure constructed from bony struts with thin level of the bone fibers, individual struts were tested in membranes. both tension and compression. Beak trabeculae from the Fig. 18 shows photographs and schematics of the toucan inner cellular structure were sectioned from beak foam by and hornbill beaks. This structure was found by Seki razor blade. The cross-section of trabeculae is elliptical or et al. (2005) to have a maximum bending moment (Brazier circular; dimensions are typically ∼200 µm in diameter and moment) that is considerably higher than if all the mass ∼1.6 mm in gauge length. The trabeculae were affixed in were concentrated in the shell as a solid hollow cylinder polymer resin mold that was allowed to harden and tested by applying the analysis developed by Karam and Gibson under tension as shown in Fig. 21(a). For compression, the (1995). Seki et al. (2005, 2006) showed that the internal cellular trabeculae were glued onto metal plates and tested as shown core serves to increase the buckling resistance of the beak and in Fig. 21(b). Dimensions of compression samples varied from demonstrated a synergism between the two components that 2.5 to 4.5 mm in gauge length; 0.09 to 0.16 mm in thickness; provides the stability in bending configuration. Thus, there is and 0.12 to 0.28 mm in width. An Instron Model 3342 with clearly an advantage in having an internal foam to support 500 N load cell and cross-head speed of 0.05 mm/min was the shell. The nature of the internal foam structure is revealed used for the trabeculae. The specimens fractured at the edge in considerable detail by micro-computerized tomography. were removed from the sampling to eliminate the effect of the Fig. 19 shows both longitudinal and cross-sections of the adhesive. Young’s modulus obtained from twenty-five tensile internal foam. The cell sizes are of the order of 1 mm. tests of trabeculae is 3.0 ± 2.2 GPa. The tensile strength was The mechanical properties of the shell are measured along well described by a Weibull distribution with a characteristic the longitudinal and transverse directions and are found to strength, σ0 = 97 MPa (Fig. 22(a)). The compressive tests be anisotropic (Fig. 20(a)). The compressive strength of the produced buckling of the struts. The response of the struts foam was established (Fig. 20(b)). It was found, as predicted, is well described by the classic Euler equation for columns that the foam in the hornbill is much stronger, by virtue subjected to compression (Fig. 22(b)); the results fluctuate of its higher density. In order to model the beak foam somewhat between fixed and pinned ends. The structure of by FEM, its compressive behavior was first evaluated; we shell and foam are imported and converted into meshes as further performed tensile and compression testing on the shown in Fig. 23. The FEM simulation of the response of trabeculae and the cortical shell to obtain the mechanical the beak was implemented by separating the shell and the properties of the foam material. Although the cortical shell interior, importing the microstructure of the bony foam with 16 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 19 – Three-dimensional structure of foam generated by VTK at distal and proximal cross-sections as well as a sagittal view of the mid-region from µ-CT scans for: (a) toucan and (b) hornbill. Source: Adapted from Seki et al., Acta Biomater. (2010).
Fig. 20 – Representative stress–strain curves for toucan and hornbill beaks: (a) external keratin (rhamphotheca) in tension; (b) internal foam in compression. Source: Adapted from Seki et al., Acta Biomater. (2010). JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 17
Fig. 21 – Mechanical testing procedure for trabeculae; (a) tensile and (b) compressive tests.
1 120 a b pinned fixed 100 0.8
80 σ = 97 MPa 0.6 0 60 0.4 40 Euler Curve Buckling stress (MPa) Buckling Failure probability Failure Euler Curve (fixed ends) (pinned ends) 0.2 20
0 0 0 50 100 150 200 0 20 40 60 80 100 Tensile strength (MPa) Slenderness ratio
Fig. 22 – Mechanical testing of individual bone fibers from cellular structure; (a) Weibull distribution from tension; (b) Euler curves (buckling stress versus slenderness ratio), results from tensile and compression testing.
a 93 µm resolution, and by bringing together and assembling Fig. 25(c). The combined action of the two components leads the two components, as shown in Fig. 23. to the synergy observed in the beak and depicted in Fig. 27. The strength of the shell, shown in Fig. 20(a) and that One sees in a clear fashion that shell+foam is stronger than of the bony struts served as input for the modeling effort, the sum of shell and foam compressed separately. whose results are illustrated in Fig. 24. This enables the Sandwich composites can be found not only in nature simulation of the compressive deformation of a segment but also in engineering materials. Gibson and Ashby (1997) of the beak. The results of the simulation (Fig. 24(a)) are describe a number of synthetic sandwich structures. There compared with actual experiment (Fig. 24(b)) and it is found are polyurethane foams (self-skinning) with higher density that the FEM model captures the most important aspects on the outer surface and lower density in the core. Most of the deformation process, including the buckling and engineering sandwich panels are made from a high-modulus tearing of the shell. Thus, a rigorous analysis coupled with face material and a low-modulus foam core. Hence, the the local mechanical property collection can simulate the toucan beak presents a novel approach to the design of response of the beak. This study is in line with current efforts these structures. Recently, a new class of materials, metallic focusing on cancellous and compact bone using mechanical foam, has been introduced and applied to make sandwich properties at the small scale and capturing the details of panels that have superior properties to polymeric foams. In the deformation and failure process (Rietbergen et al., 1995; synthetic sandwich panels, the combination of foam core Müller and Rüegsegger, 1995; Ulrich et al., 1998; Borah et al., and face materials is selected as a compromise between cost 2001; Nagaraja et al., 2004). Figs. 25 and 26, respectively, show and performance. Despite these developments, the sandwich the separate responses of the shell and cellular bone interior composites in nature are still far beyond the man-made to compression. The shell readily collapses by buckling in constructions in terms of functionalities and optimization. 18 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 23 – Conversion of CT images to FE model; (a) CT image, scanned with a resolution of 93 µm; (b) tridimensional rendering of bony foam and shell; (c) FE model of shell and foam, finally assembled to create bony beak foam.
4. Functional biological materials mechanisms acting separately or together: wet adhesion (capillarity), dry adhesion (van der Waals), and suction Biological materials exhibit a range of functional properties, (through reduced internal pressure). which have been extensively studied in the past years. We will illustrate these concepts through three examples: Noteworthy are the optical properties of the hexactinellid the gecko, the tree frog (Scynax perereca), and the abalone foot. sponge, that act as optical fibers; the brittle star, an echinoderm, changes color from black (during day) to white 4.1. The gecko foot (at night) (Aizenberg, 2010); the iridescence of butterflies, related to the nanostructure of the wing; the chameleon skin, The gecko is the stellar example of an animal that can that changes its color; the generation of current in electric apparently defy gravity by using a unique structure in the eels; the magnetic oxides embedded in the brains of pigeons foot pad. It is well known and intensively studied. However, that act as guidance systems. the mechanism by which it attaches itself is not unique. Flies, We focus here on one functional property, the ability bugs, and other taxa have developed similar devices. Fig. 28(a) to attach to surfaces. Barnacles (Berglin and Gatenholm, shows a common ladybug attached onto a flower. Fig. 28(b) 2003) and mussels (Waite and Tanzer, 1981; Waite, 1987; Bell is a SEM micrograph showing a retracted foot. One should and Gasoline, 1996) attach in a permanent manner through notice that the ladybug has quite hairy legs. Upon observation intricate processes involving chemistry. However, a number at a higher magnification (Fig. 28(c)), it is apparent that the of animals have evolved reusable attachment devices: insects, foot contains thin cylindrical rods, called setae, terminating lizards, frogs. Barnes (2007) classifies attachment devices in in spatulae, with diameters of ∼2 µm. These spatulae attach animals into: to surfaces through van der Waals forces. • Interlocking: Interlocking is the mechanism by which In the case of the gecko, which has a much bigger mass, felines climb trees. This is a strictly mechanical process the setae and spatulae are equally observed. A principal and can be accomplished by penetrating the surface with difference is the greater extent to which the setae split into sharp claws. spatulae, with diameters of ∼100 nm. The setae are arranged • Friction: Friction consists of the micro-interlocking of the bundles which have a regular pattern with channels between surfaces because of their roughness and intermolecular them. These bundles have an approximate square shape with forces between materials and requires an angle that is 10 µm side. Fig. 29 shows this in a clear manner. These below 90◦. bundles terminate at a common source and have a length of • Bonding: it involves the formation of bonds between ∼100 µm. The distal ends of the setae split up into a large the animal and the surface and has three possible number of fibrils. The terminations, called spatulae, have JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 19
Fig. 24 – Comparison of experiment and FEA; (a) deformation of foam in FEM calculation at strains of 0, −0.25, −0.5; (b) deformation of foam in experiment at strains of 0, −0.25, −0.5 strain; (c) cortical shell splitting in FEA at −0.1 strain; (d) FEM calculation at −0.5 strain, showing that the bony exterior is locally buckled and fractured. diameters between 50 and 120 nm. The scale of the gecko where γ is the work of adhesion of the two surfaces that spatulae is one order of magnitude lower than that of the produces the van der Waals force. The critical radius of ladybug. contact ac is obtained by taking: Arzt et al. (2003) and Huber et al. (2005) calculated the ∂F stress required to pull off a contact and explained the scale = 0. (11) effect. This calculation is based on the van der Waals forces ∂a combined with Hertzian contact stresses. For simplicity, This leads to spatulae are assumed to have semi-spherical extremities, as 3 a first approximation. The contact radius, a, for a spherical Fc = πRγ. (12) 2 cap of radius R in contact with a flat surface and subjected to a compressive force F is, according to Hertzian elasticity This result is, surprisingly, independent of E. More complex (e.g., Ugural and Fenster, 1987): analyses incorporate the elastic constants. In the case of 2RF attachments, only a fraction of the surface, f, is covered a = 0.88 . (9) E∗ by spatulae. The adhesion stress can be computed from Fc Johnson et al. (1971) inserted the attractive force between the considering the area of contact of each spatula to be equal 2 two bodies and obtained the expression (as quoted by Arzt, to πR . The stress required to pull off a spatula is the force F 2006): divided by the apparent area, 3 4 a 1/2 3 fγ F = E − (4πEγa) (10) σapp = (13) 3 R 2 R 20 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 25 – FEM simulation of the beak shell under compression testing; (a) FEM model of shell; (b) onset of folding; (c) buckled shell; (d) completely collapsed shell. Source: Adapted from Seki et al., MSEC (2006). where f, the fraction of the area covered by setae, is of the Brazilian tree frog is also, and surprisingly, composed of aligned nanoscale fibrils. The fibrils are sectioned into πR2 f = . (14) highly ordered hexagonal bundles (Lin, 2008). These bundles, A app described first by Ernst (1973a,b); Welsh et al. (1974) and It can be seen that the pull-off stress in Eq. (13) is inversely studied later by many others (Green, 1979; McAllister and proportional to R. Thus, the larger the mass of the biological Channing, 1983; Green and Simon, 1986) are separated by system, the smaller R has to be. For geckos, that have a mass canal-like grooves. More recent studies have been carried out of approximately 100 g, it is equal to 10 setae per µm2. The by Hanna and Barnes (1991) and Barnes et al. (2005, 2006). ladybug, on the other hand, has a mass of ∼0.2 g and a density The structure of the toe pad is depicted in the schematic of 0.05–0.2 setae per µm2. It should be mentioned that for diagram presented in Fig. 30. The diagram shows a tree extremeties that are not semi-spherical other relations apply, frog attached to a glass substrate,with an illustration of the as will be seen under Section 5. hexagonal subdivisions approximately 10 µm in diameter. These subdivisions are comprised of closely packed fibers 4.2. Tree frog approximately 100 nm in diameter. Each fiber terminates in cups of approximately 200 nm diameter (Lin, 2008). Each one The toe pad of the Brazilian tree frog (Scynax perereca) of these cups is aligned beside its neighbor forming a flat provides a splendid example of functional adhesion in surface. Fig. 31 provides a scanning electron micrograph of a nature. This animal, which lives in the moist environment single toe at low magnification with an expanded view of the of the subtropical rain forest, is able to jump from surface surface of the toe pad showing hexagonal subdivisions. A well to surface, and attach itself effectively through a variety defined circular pad of roughly 2.5 mm in diameter can be of electro/mechanical/chemical actions employed by the seen at the center of the toe. This area represents the surface materials at the surface of its toe. Its movements are much of thousands of well packed pseudo-hexagonal bundles as more dynamic than the gecko. We observed that the toe pad seen in the expanded caption of the figure. JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 21
Fig. 26 – FEM modeling of foam under uniaxial compression testing; (a) undeformed foam; (b) deformed foam. Source: Adapted from Seki et al., MSEC (2006).
Stress (MPa) Foam filled shell Fig. 28 – Ladybug attachment devices: (a) ladybug; (b) 10 retracted foot; (c) setae terminating in spatula.
Interaction effect 5 Shell+foam that exist between the hexagonal subsections. It had been 0 0 0.2 0.4 0.6 0.8 1 suggested that the fluid plays an essential role in adhesion, Strain indicating a domination of wet adhesion mechanism. It is proposed here that the contribution of molecular adhesion + Fig. 27 – Compressive stress–strain curves of foam shell through van der Waals interactions between the nanofibril and foam filled shell which show strong synergistic effect. ends and a surface may have a place in the discussion of tree Source: Adapted from Seki et al., Acta Mater. (2005). frog toe pad adhesion. Fig. 32 provides (a) top-down, and (b) cross-sectional view of an individual bundle. The tightly packed, well aligned fibers Barnes (2007) reported that the mucous glands excrete a which comprise these bundles are shown in greater detail viscous fluid which can be transported through the canals in Fig. 33. The terminating cups on neighboring fibers are 22 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
(SEM) image of the cross-section of the soft tissue. Folds can be seen in greater detail as a mechanism in which the surface area of the foot can expand and contract allowing an increase or decrease in contact surface area and providing the mechanism for the propagation of waves on the ventral surface of the pedal muscle. At higher magnification, Fig. 36(a) shows setae lining the outer surface of the tissue with a thickness of 1–2 µm. At their extremities, (Fig. 36(b)) the setae separate into nanoscale probes with hemispherical ends (c), averaging 150 nm in diameter and uniaxially aligned perpendicular to the plane of the foot tissue. It is proposed that, as in the case of the gecko, these nanofibrils create intimate contacts at the molecular level to form van der Waals interactions which can be accumulated into a formidable macroscale effect. A close view showing the alignment of these nanofibrils is shown in Fig. 37. The influence of a meniscus fluid between a fiber and a substrate is increasingly significant with decreased liquid–surface contact angle, i.e. a hydrophilic substrate would have more capillary interactions than a hydrophobic one. This is clearly seen in Fig. 38. In the case of the hydrophobic material the average pull-off force was determined to be 294 nN, remaining constant under varying humidities. If one assumes that 60 nanofibrils on a single seta are in contact with the surface, this would correspond to an adhesion force of approximately 5 nN per nanofibril. This estimate is in exact agreement with the theoretical results of 5 nN calculated using the Johnson–Kendall–Roberts equation. When the seta was tested on a hydrophilic substrate, at a relative humidity of 10%, the pull-off force was observed to be 424 nN before detachment. This represents an increased force of 130 nN relative to test on the hydrophobic substrate, which can be partially explained by the variation in surface energies for the two substrates Fig. 29 – Gecko and structure of attachment shown at (20 mJ/m2 and 55.5 mJ/m2 for the disc and silicon oxide, increasing magnifications, starting with setae in respectively). However, raising the relative humidity to 67% rectangular arrays terminating in spatulae with diameters resulted in an additional increase in pull-off force to 558 of approximately 100 nm. nN. Similar to predictions by Autumn et al. (2002) and work by Huber et al. (2005) for the gecko foot, this shows evidence of capillary interactions. The characterization of the abalone aligned closely against each other to create a smooth and foot pedal and the mechanical tests suggest that the three consistent surface. mechanisms proposed by Barnes (2007) act cooperatively (and perhaps synergistically). Suction can generate attachment 4.3. Abalone foot attachment forces as explained schematically in Fig. 39 (a). It can be shown that the detachment force F is equal to: Our group has extended the study of the structure of abalone d to the attachment forces required to separate it from a Fd = PA (15) surface (Lin et al., 2009). The detachment stresses were where P is the pressure and A is the projected area of the measured on live and healthy abalone and found to be of abalone foot on the plane of the surface of attachment. the order of 115 kPa. The pedal foot of red abalone (Haliotis Assuming that the effect of the water column is negligible, rufescens) is shown in Fig. 34. The dark pedal folds, spaced i.e., P = P , we obtain the mean attachment stress as, approximately 0.5 mm apart, are the source of locomotion atm waves used in transportation (Trueman and Hodgson, 1990; σd = Patm = 101 kPa. (16) Donovan and Carefoot, 1997). These locomotion waves have an analog in Materials Science in the dislocation. The fold Fig. 39(b,c) show schematically how the three mechanisms in the pedal propagates along the foot, generating, after can operate cooperatively to create the attachment stress its passage, a displacement equal to the length of surface on the same order of magnitude as the theoretical suction at fold. Fig. 34(b) shows an abalone supporting its own stress. The setae and nanofibrils maintain intimate contact weight via a single contact point (a human finger). Fig. 35 with any irregular surface, closing possible channels and shows a large magnification scanning electron microscopy impending water penetration. The pressure at the interface, JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 23
Fig. 30 – Schematic diagram of the structural hierarchy found in the toe pad of a Brazilian tree frog (Scynax perereca).
Fig. 31 – Scanning electron micrograph of the toe pad of a Brazilian tree frog; (a) low magnification view of single toe, (b) hexagonal subsections found on the contact surface of the toe pad.
P0, is equal to Patm when no external detachment force is effectively eliminates suction. It is proposed that capillarity applied. As Fd increases, P0 decreases. Once it becomes zero, and van der Waals forces can maintain the intimate contact detachment occurs. Fig. 39(c) shows the situation for a non- between the ventral side of the foot pedal and the attachment conforming material: A continuous fluid path to the interface surface; in this manner the suction force can reach and even region ensures pressure equilibration around the animal and exceed PatmA. 24 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 32 – Scanning electron micrographs of hexagonal subdivisions: (a) top-down view; (b) side view.
Fig. 34 – The pedal foot of the red abalone: (a) optical image of bottom surface of foot; (b) abalone supporting its own hanging weight through single contact point. Source: Adapted from Lin et al., Acta Mater. (2009).
and with the ever better understanding of material–organism interaction. But the third, bioinspired design, poses the greatest challenge. The development and implementation of concepts learned from nature can exist at two levels:
• Design, using concepts from nature but applying synthetic materials and conventional processing methods. • Molecular-based bioinspired structures. In this approach, we mimic nature all the way down to the molecular level, using biological approach of self-assembly and molecular Fig. 33 – High magnification of individual fibers engineering. comprising the larger hexagonal subdivisions. The first approach is much more conventional and has been implemented successfully in a number of applications. 5. Bioinspired materials and structures We will focus on only a few to illustrate this concept. From the historical and commercial success viewpoint, the discovery This is the most difficult of the three areas delineated by George de Mistral of burrs that stuck stubbornly to his in Section 1, both experimentally and analytically. The pants and hunting dog is illustrative of the approach. Fig. 40(a) study of biological materials is benefitting from the modern shows the tip of a curved burr found in European countryside. analytical, characterization, and computational tools and by These tips have characteristic hooks which render them the ever increasing numbers of investigators combing the particularly attachable to fur in animals and, more recently, field, globally. Bio and biomedical materials are in synergy loops in clothing. The plants use this strategy to spread the with advances made in materials synthesis and processing, seeds around. This principle was used by George de Mistral JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 25
Fig. 37 – Nanofibrils uniaxially aligned along the outer surface of the foot tissue. Fig. 35 – Scanning electron microscopy of foot tissue Source: Adapted from Lin et al., Acta Mater. (2009). cross-section, the top of the image represents the contact surface of the foot. Source: Adapted from Lin et al., Acta Mater. (2009). in the development of VELCRO (from VELours CROchet). Fig. 40(b) shows synthetic hooks embedded in the fabric. They were initially loops with ∼200 µm diameter, on the same order
Fig. 36 – SEM characterization of abalone foot tissue: (a) seta lining the outer surface of the foot; (b) nanofibers uniaxially aligned on seta; (c) single nanofiber with hemispherical tip. Source: Adapted from Lin et al., Acta Mater. (2009). 26 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
600 hydrophilic silica a 550 hydrophobic material
400 capillary van der Waals 350 pull-off force [nN] pull-off force
250 van der Waals 200 0 10203040506070 relative humidity [%]
Fig. 38 – Pull-off force as a function of relative humidity of b a single seta on a hydrophobic and a hydrophilic substrate. Source: Adapted from Lin et al., Acta Mater. (2009).
Fig. 40 – SEM micrographs showing the microstructure of (a) a seed-bearing burr; (b,c) hooks and loops in Velcro.
Fig. 39 – Schematic representation of how suction might generate attachment forces. shows a lotus leaf floating on water. The water at its top does Source: Adapted from Lin et al., Acta Mater. (2009). not wet it, but concentrates into small areas by virtue of the hydrophobicity of the surface. This is necessary to clean the lotus leaf and ensure its flotation. Drops of water will just roll as burrs, which are severed, separating the regions A and B in off the leaf (shown in the right photograph of figure). Fig. 40(b), which were initially connected. The loop portion of The surface of the lotus leaf has small pillars of a Velcro is shown in Fig. 40(c). It is an irregular array of fibers few micrometers height and spaced ∼20 µm (Fig. 41(b)). with ∼50 µm thickness. These are, in turn, covered by smaller scale protrusions, Another application that is generating considerable with dimensions of ∼0.2–1 µm. These are, in their turn, excitement is the use of the hydrophobicity of the lotus flower covered with wax. The net result is that the angle of contact for self-cleaning surfaces. This effect was studied by Barthlott between water droplets and the surface is dramatically and Ehler (1977), Barthlott (1990), Barthlott and Neinhuis increased. Hydrophilic surfaces have contact angles below (1997) and recently reviewed by Koch et al. (2009). Fig. 41(a) 90◦, whereas hydrophobic surfaces have angles above 90◦. JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 27
Fig. 41 – The lotus leaf effect: (a) lotus leaf upon which water does not wet; (b) schematic of the surface showing two scales of protrusions which lead to an angle greater than 90◦.
Fig. 42 – (a) SEM micrographs showing micro-pillar arrays with cylindrical and mushroom-like geometries; (b) Pull-off strength increases with decreasing pillar radius. Source: Adapted from Del Campo et al. (2007b), Greiner et al. (2007). 28 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Fig. 44 – (a) Fracture toughness for lamellar and brick-and-mortar composites compared with that for Al2O3 and PMMA. Both types of composites are significantly tougher than their constituents. (b) The composites show significant rising R-curve behavior due to micro- and nanoscale toughening mechanisms. Source: Adapted from Munch et al., Science (2008).
Fig. 43 – Microstructure of abalone nacre-inspired microwave antennae which help to keep them dust free and Al O /PMMA composites in (a) lamellar and (b) 2 3 decrease the buildup of ice and snow. brick-and-mortar forms produced by freeze casting The gecko attachment principle has given rise to extensive techniques; (c) bridge between two tile layers. research in the hope of creating structures that have Source: Launey et al., Acta Mater. (2009). reversible attachment properties. We illustrate here one successful program that has generated surfaces with pillars that have demonstrated excellent attachment capability. For the lotus, this angle can be as high as 160◦, and it is Arzt et al. (2003), Huber et al. (2005), Del Campo et al. therefore called super-hydrophobic. This hydrophobicity has (2007a,b), Greiner et al. (2007) and Greiner et al. (2009) have an important effect: water droplets, almost perfect spheres, made significant progress in mimicking the structure of the can roll over the surface. When they do this, they pick up gecko foot by using polydimethylsiloxane (PDMS) surfaces, dust particles which decrease their surface energy by being patterned with fibrils having different termination shapes. absorbed into the water droplets. Thus, the surface cleans Shown in Fig. 42(a) are flat and mushroom shapes. The itself. In 1999, a commercial and very successful product was mushroom shape had a pull-off force approximately 20 times launched: the facade paint Lotusan has been applied on more that for surfaces patterned with fibrils having simple semi- than 500,000 buildings worldwide so far. Other applications spherical cap geometry. are self-cleaning glasses installed in the sensors of traffic For flat and mushroom-shaped fibrils, exceptionally high control units on German highways and coatings applied to adhesion strength values, approaching and exceeding that of JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 29 the natural attachment of the gecko, were found. The sizes of 6. Conclusions the pillars were also changed and it was found that the pull- off force of flat pillars increased with the decrease in radius, Given below are some broad conclusions which show the i.e., the force is proportional to R−1/2. These results are shown principal attributes of the emerging field of biological and in Fig. 42(b). The size dependence of Eq. (13) applies to semi- bioinspired materials in MSE. spherical caps where the JKR equation can be applied directly. Assuming geometrical similarity, the pull off stress should • We are trying to understand the structure–property be proportional to 1/R. In the case of a flat punch, the JKR relations in biological materials, all the way from the nano −1/2 equation does not apply and σ is proportional to R (Chan to the structural level. et al., 2007). • The connections between the different structural levels The recent development of a gecko-inspired tissue and the assembly processes used by organisms to develop adhesive for biomedical applications by Langer, Karp, and co- their structures are being investigated using the powerful workers (Mahdavi et al., 2008) also has great potential. They analytical, experimental, and computational arsenal of demonstrated that gecko-inspired arrays of pillars of PGSA MSE. (polyglycerol sebacate acrylate) provided attachment under • We illustrated a number of essential concepts with, water. This tape is proposed as a biodegradable polymer primarily, the results of our research. Thus, this overview adhesive to tissue. The adhesion was tested in vitro to is limited in scope and only captures a small fraction of porcine intestine and in vivo to rat abdominal muscle. Carbon the work being carried out. nanotube arrays are also being proposed to form fibrilar • Recognizing the limited supply of materials available in arrays and have self-cleaning properties due to extreme biological systems and the narrow range of temperatures hydrophobicity (Sethi et al., 2008). The effects of angled in which synthesis and processing takes place, we fibrilar attachments have also been investigated and it was should use the design principles of nature to amplify demonstrated to have an important bearing. their effectiveness. Our current technological capabilities At UC Berkeley and Lawrence Berkeley National Lab, a re- can expand the biological manufacturing principles search group led by Ritchie and Tomsia (Deville et al., 2006a,b; to a broader range of temperatures, pressures, and Munch et al., 2008; Launey et al., 2009, 2010b) mimicked the compositions, while retaining the essential features. abalone’s toughening mechanisms by combining aluminum • Biomimicking is evolving from purely synthetic processes oxide and polymethyl methacrylate (PMMA). They used an using design concepts from nature (such as, for instance, ice-templated manufacturing technique to create the lamel- VELCRO) to molecular-based processing in which self- lar structure in alumina and were able to achieve outstanding assembly and other unique natural processes of nature are mechanical properties. The structure has several of the basic used. components of nacre as can be seen by comparing Fig. 43(a) • with Fig. 16(b) and 17. The tiles are present (alumina instead We foresee continued and expanded activity in the field of aragonite) with the organic interlayer being replaced by of biological and bioinspired materials as large numbers PMMA. It should be noticed that their thickness is consid- of investigators globally explore natural materials and erably higher than in nacre, ∼10 µm versus ∼0.5 µm. There discover new structural designs and concepts. This are bridges between the tiles, shown in Fig. 16(b) and 43(b). expansion in our understanding will be (and already is) paralleled by a whole array of novel synthesis and The final product is a solid ceramic-based laminate compos- processing methods to produce bioinspired materials and ite with a high yield strength and fracture toughness. For a structures. Aizenberg’s (2010) recent MRS lecture is a 80% Al2O3–20% PMMA laminate, a tensile strength of 200 MPa stellar example of this effort. and fracture toughness of 30 MPa.m1/2 are obtained. These values represent specific properties comparable to those of aluminum alloys. It should be noted that this is accom- plished with the majority being alumina. The resistance to crack propagation (R curve behavior) is shown in Fig. 44(b). Acknowledgements The increase in toughness with crack propagation is obvious. 1/2 The curve rises to KIc = 30 MPa m . This is in stark con- This research was supported by The National Science trast with monolithic alumina, which has a flat curve with Foundation Division of Materials Research, Biomaterials 1/2 KIc = 1 MPa m . One unique aspect of the architecture Program, Grant DMR 0510138. We thank Profs. J. McKittrick, of this bioinspired material is that when it has the abalone C.T. Lim, and R.O. Ritchie for helpful discussions. We also brick-and-mortar structure with bridges between the tiles, thank Eddie Kisfaludi for taking care of the abalone, S.G. the toughness is increased over the purely lamellar struc- Bodde for providing figures, and Ryan Anderson (CALIT2) and ture (∼15 MPa m1/2). The more conventional simple laminate C.T. Wei for the use of the SEM. We thank the referees for structure is definitely less tough than the new material. This their thoughtful comments which enriched this manuscript. example illustrates the potential of (a) understanding and (b) In particular, the fourth paragraph in the Introduction is taken mimicking biological materials. from the comments by one of them. 30 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
REFERENCES Chen, P.-Y., Lin, A.Y.M., Lin, Y.S., Seki, Y., Bodde, S.G., Stokes, A.G., McKittrick, J., Meyers, M.A., 2008b. Structural biological materials: overview of current research. JOM 60, 23–32. Chen, P.-Y., Lin, A.Y.M., McKittrick, J., Meyers, M.A., 2008c. Aizenberg, J., 2010. New nanofabrication strategies: inspired by Structure and mechanical properties of crab exoskeletons. mineralization. MRS Bull. 35, 323–330. Acta Biomater. 4, 587–596. Arzt, E., 2006. Biological and artificial attachment devices: Lessons Chen, P.-Y., Stokes, A.G., McKittrick, J., 2009. Comparison of for materials scientists from flies and geckos. Mater. Sci. Eng. structure and mechanical properties of bovine femur bone and C 26, 1245–1250. antlers of the North American elk (Cervus canadensis). Acta Arzt, E., Gorb, S., Spolenak, R., 2003. Evidence for van der Waals Biomater. 5, 693–706. adhesion in gecko setae. Proc. Natl. Acad. Sci. USA 100, 10603–10606. Del Campo, A., Greiner, C., Alvarez, I., Arzt, E., 2007a. Patterned Surfaces with Pillars with 3D Tip Geometry Mimicking Autumn, K., Sitti, M., Liang, Y.A., Peattie, A.M., Hansen, W.R., Bioattachment Devices. Adv. Mater. 19, 1973–1977. Sponberg, S., Kenny, T.W., Fearing, R., Israelachvili, J.N., Full, R.J., 2002. Evidence for van der Waals adhesion in gecko setae. Del Campo, A., Greiner, C., Alvarez, I., Arzt, E., 2007b. Contact Proc. Natl. Acad. Sci. USA 99, 12252–12256. shape controls adhesion of bioinspired fibrillar surfaces. Langmuir 23, 10235–10243. Barnes, W.J.P., 2007. Functional morphology and design con- straints of smooth adhesive pads. MRS Bull. 32, 479–485. Deville, S., Saiz, E., Nalla, R.K., Tomsia, A.P., 2006a. Freezing as a Barnes, W.J.P., Perez-Goodwyn, P., Gorb, S.N., 2005. Mechanical path to build complex composites. Science 311, 515–518. properties of the toe pads of the tree forg, Litoria caerulea. Deville, S., Saiz, E., Tomsia, A.P., 2006b. Freeze casting of hydrox- Comp. Biochem. Physiol. A 141, S145. yapatite scaffolds for bone tissue engineering. Biomaterials 27, Barnes, W.J.P., Oines, C., Smith, J.M., 2006. Whole animal 5480–5489. measurements of shear and adhesive forces in adult tree frogs: Donovan, D.A., Carefoot, T.H., 1997. Locomotion in the abalone insights into underlying mechanisms of adhesion obtained Haliotis kamtschatkana: pedal morphology and cost of trans- from studying the effects of size and shape. J. Comp. Physiol. port. J. Exp. Biol. 200, 1145–1153. A 192, 1179–1191. Ehrlich, H., 2010. Chitin and collagen as universal and alternative Barthlott, W., 1990. Scanning electron microscopy of the templates in biomineralization. Int’l. Geology Rev. 52, 661–699. epidermal surface in plants. In: Claugher, D. (Ed.), Application Ernst, V.V., 1973a. The digital pads of the tree frog Hyla cinerea. I. of the Scanning EM in Taxonomy and Functional Morphology, The epidermis. Tissue Cell 5, 83–96. Systematics Association’s Special Volume. Clarendon Press, Ernst, V.V., 1973b. The digital pads of the tree frog Hyla cinerea. II. Oxford, pp. 69–94. The mucous glands. The epidermis. Tissue Cell 5, 97–104. Barthlott, W., Ehler, N., 1977, Raster-Elektronenmikroskopie der Espinosa, H.D., Rim, J.E., Barthelat, F., Buehler, M.J., 2009. Merger Epidermis-Oberflächen von Spermatophyten. Tropische und of structure and material in nacre and bone — Perspectives on subtropische Pflanzenwelt (Akad. Wiss. Lit. Mainz) 19, 110. de novo biomimetic materials. Prog. Mater. Sci. 54, 1059–1100. Barthlott, W., Neinhuis, C., 1997. The purity of sacred lotus or Fratzl, P., Weinkamer, R., 2007. Nature’s hierarchical materials. escape from contamination in biological surfaces. Planta 202, Prog. Mater. Sci. 52, 1263. 1–8. Fratzl, P. (Ed.), 2008. Collagen: Structure and Mechanics. Springer, Belcher, A.M., Wu, X.H., Christensen, R.J., Hansma, P.K., Stucky, New York. G.D., Morse, D.E., 1996. Control of crystal phase switching Fritz, M., Belcher, A.M., Radmacher, M., Walters, D.A., Hansma, and orientation by soluble mollusc-shell proteins. Nature 381, P.K., Strucky, G.D., Morse, D.E., Mann, S., 1994. Flat pearls 56–58. from biofabrication of organized composites on inorganic Bell, E.C., Gasoline, J.M., 1996. Mechanical design of mussel substrates. Nature 371, 49. byssus: material yield enhances attachment strength. J. Exp. Fung, Y.C., 1993. Biomechanics: Mechanical Properties of Living Biol. 199, 1005–1017. Tissues, 2nd edition. Springer-Verlag, New York. Berglin, M., Gatenholm, P., 2003. The barnacle adhesive plaque: morphological and chemical differences as a response to Gao, H., Ji, B., Jäger, I.L., Arzt, E., Fratzl, P., 2003. Materials become substrate properties. Colloids Surf. 28, 107–117. insensitive to flaws at nanoscale: lessons from nature. Proc. Natl. Acad. Sci. USA 100, 5597–5600. Borah, B., Gross, G., Dufresne, T., Smith, T., Cookman, M., Chmielewski, P., Lundy, M., Hartke, J., Sod, E., 2001. Three- Gao, H., 2006. Application of fracture mechanics concepts to dimensional microimaging (MRµl and µCT), finite element hierarchical biomechanics of bone and bone-like materials. modeling, and rapid prototyping provide unique insights into Intl. J. Fracture. 138, 101–137. bone architecture in osteoporosis. Anatom. Rec. 264, 101–110. Gibson, L.J., Ashby, M.F., 1997. Cellular Solids: Structure and Prop- Buehler, M.J., 2007. Nano- and micromechanical properties of erties, 2nd edition. Cambridge University Press, Cambridge. hierarchical biological materials and tissues. J. Mater. Sci. Green, D.M., 1979. Tree frog toe pads: comparative surface 8765–8770. morphology using scanning electron microscopy. Can. J. Zool. Buehler, M.J., Keten, S., Ackbarow, T., 2008. Theoretical and com- 57, 2033–2046. putational hierarchical nanomechanics of protein materials: Green, D.M., Simon, P., 1986. Digital microstructure in ecologically Deformation and fracture. Prog. Mater. Sci. 53, 1101–1241. diverse sympatric microhylid frogs, genera Cophixalus and Chan, E.P., Greiner, C., Arzt, E., Crosby, A.J., 2007. Designing model Sphenophryne (Amphibia: Anura). Papua New Guinea. Aust. J. systems for enhanced adhesion. MRS Bull. 32, 496–503. Zool. 34, 135–145. Checa, A.G., Cartwright, J.H.E., Willinger, M.G., 2009. The key role Greiner, C., Arzt, E., Del Campo, A., 2009. Hierarchical gecko-like of the surface membrane in why gastropod nacre grows in adhesives. Adv. Mater. 21, 479–482. towers. Proc. Natl. Acad. Sci. USA 106, 38–43. Greiner, C., Del Campo, A., Arzt, E., 2007. Adhesion of bioinspired Chen, P.-Y., Lin, A.Y.M., Lin, Y.S., Seki, Y., Stokes, A.G., Peyras, J., micro-patterned surfaces: effect s of pillar radius, aspect ratio, Olevsky, E.A., Meyers, M.A., McKittrick, J., 2008a. Structure and and preload. Langmuir 23, 3495–3502. mechanical properties of selected biological materials. J. Mech. Hanna, G., Barnes, W.J.P., 1991. Adhesion and detachment of the Behav. Biomed. Mater. 1, 208–226. toe pads of treefrogs. J. Exp. Biol. 155, 103–125. JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) – 31
Huber, G., Mantz, H., Spolenak, R., Mecke, K., Jacobs, K., Gorb, S.N., McKittrick, J., Chen, P.-Y., Tombolato, L., Novitskaya, E.E., Trim, Arzt, E., 2005. Proc. Natl. Acad. Sci. USA 102, 16293–16296. W., Lin, Y.S., Hirata, G.A., Olevsky, E.A., Horstemeyer, M.F., Jäger, I., Fratzl, P., 2000. Mineralized collagen fibrils: a mechanical Meyers, M.A., 2010. Energy absorbent natural materials and model with a staggered arrangement of mineral particles. bio-inspired design strategies: A review. Mater. Sci. Eng. C 30, Biophys. J. 79, 1737–1746. 331–342. Ji, B., Gao, H., 2004. Mechanical properties of nanostructure of Meyers, M.A., Lin, A.Y.M., Seki, Y., Chen, P.-Y., Kad, B., Bodde, S.G., biological materials. J. Mech. Phys. Solids 52, 1963–1990. 2006. Structural biological composites: an overview. JOM 58, Johnson, K.L., Kendall, K., Roberts, A.D., 1971. Surface energy 35–41. and the contact of elastic solids. Proc. Roy. Soc. London 324, Meyers, M.A., Chen, P.-Y., Lin, A.Y.M., Seki, Y., 2008a. Biological 301–313. materials: structure and mechanical properties. Prog. Mater. Kamat, S., Su, X., Ballarini, R., Heuer, A.H., 2000. Structure basis Sci. 53, 1–206. for the fracture toughness of the shell of the conch Strombus Meyers, M.A., Lin, A.Y.M., Chen, P.-Y., Muyco, J., 2008b. Mechanical gigas. Nature 405, 1036–1040. strength of abalone nacre: role of the soft organic layer. J. Mech. Kamat, S., Kessler, H., Su, X., Ballarini, R., Nassirou, M., Heuer, Behav. Biomed. Mater. 1, 76–85. A.H., 2004. Fracture mechanisms of the Strombus gigas conch Meyers, M.A., Lim, C.T., Li, A., Hairul Nizam, B.R., Tan, E.P.S., Seki, shell: II-micromechanics analyses of multiple cracking and Y., McKittrick, J., 2009. The role of organic intertile layer in large-scale crack bridging. Acta Mater. 52, 2395–2406. abalone nacre. Mater. Sci. Eng. C. 29, 2398–2410. Karam, G.N., Gibson, L.J., 1995. Elastic buckling of cylindrical shells Meyers, M.A., Lin, Y.S., Olvesky, E.A., Chen, P.-Y., 2010. Battle in with elastic cores-I: analysis. Int. J. Solids Struct. 32, 1259–1283. the Amazon: Arapaima (Pirarucu) vs. Serrasalminae (Piranha) Koch, K., Bhushan, B., Barthlott, W., 2009. Multifunctional surface (in preparation). structures of plants: An inspiration for biomimetics. Prog. Müller, R., Rüegsegger, P., 1995. Three-dimensional finite element Mater. Sci. 54, 137–178. modelling of non-invasively assessed trabecular bone struc- Launey, M.E., Munch, E., Alsem, D.H., Barth, H.D., Saiz, E., Tomsia, tures. Med. Eng. Phy. 17, 126–133. A.P., Ritchie, R.O., 2009. Designing highly toughened hybrid composites through nature-inspired hierarchical complexity. Munch, E., Launey, M.E., Alsem, D.H., Saiz, E., Tomsia, A.P., Ritchie, Acta Mater. 57, 2919–2932. R.O., 2008. Tough bio-inspired hybrid materials. Science 322, Launey, M.E., Chen, P.-Y., McKittrick, J., Ritchie, R.O., 2010a. 1515–1520. Mechanistic aspects of the fracture toughness of elk antler Nagaraja, S., Couse, T.L., Guldberg, R.E., 2004. Trabecular bone bone. Acta Biomater. 6, 1505–1514. microdamage and microstructural stresses under uniaxial Launey, M.E., Munch, E., Alsem, D.H., Saiz, E., Tomsia, A.P., Ritchie, compression. J. Biomech. 38, 707–716. R.O., 2010b. A novel biomimetic approach to the design of Nalla, R.K., Kinney, J.H., Ritchie, R.O., 2003. Mechanistic fracture high-performance ceramic/metal composites. J. R. Soc. Inter. criteria for the failure of human cortical bone. Nature Mater. 2, 7, 741–753. 164. Lin, A.Y.M., Structural and functional biological materials: abalone Nalla, R.K., Kruzic, J.J., Kinney, J.H., Ritchie, R.O., 2005. Mechanistic nacre, sharp materials, and abalone foot adhesion, Doctoral aspects of fracture and R-curve behavior in human cortical Dissertation, U. C. San Diego, 2008. bone. Biomaterials 26, 217. Lin, A.Y.M., Meyers, M.A., 2005. Growth and structure in abalone Rho, J.Y., Kuhn-Spearing, L., Zioupos, P., 1998. Mechanical shell. Mater. Sci. Eng. A 290, 27–41. properties and the hierarchical structure of bone. Med. Eng. Lin, A.Y.M., Chen, P.-Y., Meyers, M.A., 2008. The growth of nacre in Phys. 20, 92. the abalone shell. Acta Biomater. 4, 131–138. Rietbergen, B.V., Weinas, H., Huiskes, R., Odgaardt, A., 1995. A Lin, A.Y.M., Meyers, M.A., 2009. The interfacial shear strength in new method to determine trabecular bone elastic properties abalone nacre. J. Mech. Behav. Biomed. Mater. 2, 607–612. and loadin using micromechanical finite element models. J. Lin, A.Y.M., Brunner, R., Chen, P.-Y., Talke, F.E., Meyers, M.A, 2009. Biomech. 12, 69–81. Underwater adhesion of abalone: The role of van der Waals Sarikaya, M., Gunnison, K.E., Yasrebi, M., Aksay, J.A., 1990. and capillary forces. Acta Mater. 57, 4178–4185. Mechanical property-microstructural relationships in abalone Lopez, M.I., Chen, P.-Y., McKittrick, J., Meyers, M.A., 2010. Growth shell. Mater. Res. Soc. 174, 109–116. of nacre in abalone: Seasonal and feeding effect. Mater. Sci. Saunders, M., Kong, C., Shaw, J.A., Macey, D.J., Clode, P.L., 2009. Eng. C, in press (doi:10.1016/j.msec.2010.09.003). Characterization of biominerals in the radula teeth of the Lowenstam, H.A., Weiner, S., 1989. On Biomineralization. Oxford chiton, Acanthopleura hirtosa. J. Struct. Biol. 167, 55–61. University Press, New York. Seki, Y., Schneider, M.S., Meyers, M.A., 2005. Structure and Mahdavi, A., Ferreira, L., Sundback, C., Nichol, J., Chan, E., Carter, mechanical properties of the toucan beak. Acta Mater. 53, D., Bettinger, C., Patanavanich, S., Chignozha, L., Joseph, E., 5281–5296. Galakatos, A., Pryor, A., Pomerantseva, I., Masiakos, P., Faquin, Seki, Y., Kad, B., Benson, D., Meyers, M.A., 2006. The toucan beak: W., Zumbuehl, A., Hong, S., Borenstein, J., Vacanti, J., Langer, Structure and mechanical response. Mater. Sci. Eng. C 26, R., Karp, J., 2008. A biodegradable and biocompatible gecko- 1412–1420. inspired adhesive. Proc. Natl. Acad. Sci. USA 105, 2307–2312. Mann, S., 2001. Biomineralization: Principles and Concepts in Seki, Y., Bodde, S.G., Meyers, M.A., 2010. Toucan and hornbill Bioinorganic Materials Chemistry. Oxford University Press, beaks: a comparative study. Acta Biomater. 6, 331–343. New York. Sethi, S., Ge, L., Ajayan, P.M., Dhinojwala, A., 2008. Gecko-inspired Mann, S., Archibals, D.D., Didymus, J.M., Douglas, T., Heywood, carbon nanotube based self cleaning adhesives. Nano Lett. 8, B.R., Meldrum, F.C., Reeves, N.J., 1993. Crystallization and 822–825. inorganic-organic interfaces — biominerals and biomimetic Shen, X., Belcher, A.M., Hansma, P.K., Stucky, G.D., Morse, D.E., synthesis. Science 261, 1286–1292. 1997. Molecular cloning and characterization of Lustrin A, a Mayer, G., 2005. Rigid biological systems as models for synthetic matrix protein from shell and pearl nacre of Haliotis rufescens. composites. Science 310, 1144–1147. J. Biol. Chem. 272, 32472–32481. McAllister, A., Channing, L., 1983. Comparisons of toe pads of Song, F., Zhang, X.H., Bai, Y.L., 2002. Microstructure and some Southern African climbing frogs. S. Afr. J. Zool. 18, characteristics in the organic matrix layers of nacre. J. Mater. 110–114. Res. 17, 1567–1570. 32 JOURNALOFTHEMECHANICALBEHAVIOROFBIOMEDICALMATERIALS ( ) –
Song, F., Soh, A.K., Bai, Y.L., 2003. Structural and mechanical Waite, J.H., Tanzer, M.L., 1981. Polyphenolic substance of properties of the organic matrix layers of nacre. Biomaterials Mytilus edulis — novel adhesive containing L-DOPA and 24, 3623. hydroxyproline. Science 212, 1038. Stella, J.A., D’Amore, A., Wagner, W.R., Sacks, M.S., 2010. On Waite, J.H., 1987. Nature’s underwater adhesive specialist. Int. J. the biomechanical function of scaffolds for engineering load- Adhes. Adhes. 7, 9. bearing soft tissues. Acta Biomater. 6, 2365–2381. Weaver, J.C., Wang, Q., Miserez, A., Tantuccio, A., Stromberg, Tombolato, L., Novitskaya, E.E., Chen, P.-Y., Sheppard, F.A., R., Bozhilov, K.N., Maxwell, P., Nay, R., Heier, S.T., DiMasi, McKittrick, J., 2010. Microstructure, elastic and fracture E., Kisailus, D., 2010. Analysis of an ultra hard magnetic properties of horn keratin. Acta Biomater. 6, 319–330. biomineral in chiton radular teeth. Mater. Today 13, 42–52. Trueman, E.R., Hodgson, A.N., 1990. The fine structure and Weiner, S., Addadi, L., 1997. Design strategies in mineralized function of the foot of Nassarius krausslanus, a gastropod biological materials. J. Mater. Chem. 7, 689–702. moving by ciliary locomotion. J. Moll. Stud. 56, 221–228. Weiner, S., Wagner, H.D., 1998. The material bone: structure Ugural, A.C., Fenster, S.K., 1987. Advanced Strength and Applied mechanical function relations. Annu. Rev. Mater. Sci. 28, 271. Elasticity. Prentice Hall, New Jersey. Welsh, U., Storch, V., Fuchs, W., 1974. The fine structure of the Ulrich, D., Rietbergen, B.V., Weinas, H., Regsegger, P., 1998. Finite digital pads of rhacophorid tree frogs. Cell Tissue Res. 148, element analysis of trabecular bone structure: A comparison of 407–416. image-based meshing techniques. J. Biomech. 31, 1187–1192. Yang, Q.D., Cox, B.N., Nalla, R.K., Ritchie, R.O., 2006. Fracture Vincent, J.F.V., Currey, J.D. (Eds.), 1980. Mechanical Properties of length scales in human cortical bone: The necessity of Biological Materials. Cambridge University Press, Cambridge. nonlinear fracture models. Biomaterials 27, 2095. Vincent, J.F.V., 1991. Structural Biomaterials. Princeton University Yao, H., Gao, H., 2008. Multi-scale cohesive laws in hierarchical Press, New Jersey. materials. Intl. J. Solids Struct. 45, 3627–3643.